Table 46. Stress Corrosion of 400 Series Stainless Steels 



Alloy 



Stress 

 (ksi) 



Percent 



Yield 



Strength 



Exposure 

 (day) 



Depth 

 (ft) 



Number of 

 Specimens 

 Exposed 



Number 

 Failed 



Source" 



AISI 405 



43 



75 



403 



6,780 



3 







CEL (4) 



AIS1 405 



20 



35 



197 



2,340 



3 







CEL (4) 



AISI 405 



29 



50 



197 



2,340 



3 







CEL (4) 



AISI 405 



43 



75 



197 



2,340 



3 







CEL (4) 



AISI 405 



43 



75 



402 



2,340 



3 







CEL (4) 



AISI 410 



47 



30 



403 



6,780 



3 







NADC (7) 



AISI 410 



116 



75 



403 



6,780 



3 







NADC (7) 



AISI 410 



47 



30 



197 



2,340 



3 







NADC (7) 



AISI 410 



116 



75 



197 



2,340 



3 







NADC (7) 



AISI 410 



47 



30 



402 



2,370 



3 







NADC (7) 



AISI 410 



24 



50 



402 



2,370 



3 







CEL (4) 



AISI 410 



116 



75 



402 



2,370 



3 







NADC (7) 



AISI 410 



36 



75 



402 



2,370 



3 







CEL (4) 



AISI 410 



120 



- 



402 



2,370 



3 







NADC (7) 



AISI 430 



- 



30 



403 



6,780 



3 







NADC (7) 



AISI 430 



- 



75 



403 



6,780 



3 







NADC (7) 



AISI 430 



- 



30 



197 



2,340 



3 







NADC (7) 



AISI 430 



- 



75 



197 



2,340 



3 







NADC (7) 



AISI 430 



- 



30 



402 



2,370 



3 







NADC (7) 



AISI 430 



27 



50 



402 



2,370 



3 







CEL (4) 



AISI 430 



- 



75 



402 



2,370 



3 







NADC (7) 



AISI 430 



41 



75 



402 



2,370 



3 







CEL (4) 



'Numbers refer to references at end of report. 



164 



